#------------------------------------------------------------------------------
#$Date: 2019-11-23 01:13:07 +0200 (Sat, 23 Nov 2019) $
#$Revision: 231741 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/34/63/4346354.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4346354
loop_
_publ_author_name
'Chen, Hong'
'Zhao, Huishuang'
'Yu, Zheng-Bao'
'Wang, Lei'
'Sun, Licheng'
'Sun, Junliang'
_publ_section_title
;
 Construct Polyoxometalate Frameworks through Covalent Bonds.
;
_journal_issue                   17
_journal_name_full               'Inorganic chemistry'
_journal_page_first              8699
_journal_page_last               8704
_journal_paper_doi               10.1021/acs.inorgchem.5b01326
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'C2 H6 B12 O33 V5'
_chemical_formula_weight         942.49
_space_group_IT_number           65
_space_group_name_Hall           '-C 2 2'
_space_group_name_H-M_alt        'C m m m'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_H-M   'C m m m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            16
_cell_length_a                   37.4162(13)
_cell_length_b                   39.2677(11)
_cell_length_c                   16.5126(6)
_cell_measurement_temperature    100(2)
_cell_volume                     24261.1(14)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0777
_diffrn_reflns_av_sigmaI/netI    0.0590
_diffrn_reflns_limit_h_max       43
_diffrn_reflns_limit_h_min       -44
_diffrn_reflns_limit_k_max       46
_diffrn_reflns_limit_k_min       -46
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            66313
_diffrn_reflns_theta_full        25.03
_diffrn_reflns_theta_max         25.03
_diffrn_reflns_theta_min         3.22
_exptl_absorpt_coefficient_mu    0.803
_exptl_absorpt_correction_T_max  0.9028
_exptl_absorpt_correction_T_min  0.7139
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
;
_exptl_crystal_density_diffrn    1.032
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             7312
_exptl_crystal_size_max          0.45
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.13
_refine_diff_density_max         1.671
_refine_diff_density_min         -1.018
_refine_diff_density_rms         0.119
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.066
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     518
_refine_ls_number_reflns         11463
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.066
_refine_ls_R_factor_all          0.1129
_refine_ls_R_factor_gt           0.0888
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1625P)²+52.7064P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2596
_refine_ls_wR_factor_ref         0.2741
_reflns_number_gt                8173
_reflns_number_total             11463
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5b01326_si_003.cif
_cod_data_source_block           a2sq3
_cod_original_sg_symbol_H-M      Cmmm
_cod_database_code               4346354
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
V1 V 0.31727(3) 0.0000 0.23104(7) 0.0342(3) Uani 1 2 d S . .
V2 V 0.36707(3) 0.0000 0.09344(8) 0.0351(3) Uani 1 2 d S . .
V3 V 0.24221(3) 0.0000 0.27865(8) 0.0411(4) Uani 1 2 d S . .
V4 V 0.16337(4) 0.0000 0.23033(8) 0.0430(4) Uani 1 2 d S . .
V5 V 0.11471(4) 0.0000 0.09361(8) 0.0455(4) Uani 1 2 d S . .
O1 O 0.34001(10) 0.03208(9) 0.1570(2) 0.0373(9) Uani 1 1 d . . .
O2 O 0.27732(10) 0.03193(9) 0.2417(2) 0.0431(9) Uani 1 1 d . . .
O3 O 0.36168(14) 0.03100(11) 0.0000 0.0360(12) Uani 1 2 d S . .
O4 O 0.20424(10) 0.03193(11) 0.2391(2) 0.0467(10) Uani 1 1 d . . .
O5 O 0.14183(10) 0.03252(10) 0.1572(2) 0.0440(9) Uani 1 1 d . . .
O6 O 0.24002(11) 0.08095(11) 0.2155(3) 0.0566(12) Uani 1 1 d . . .
O7 O 0.12025(14) 0.03213(15) 0.0000 0.0453(13) Uani 1 2 d S . .
O8 O 0.34832(12) 0.08220(9) 0.0698(2) 0.0454(10) Uani 1 1 d . . .
O9 O 0.34964(11) 0.08830(10) 0.2144(2) 0.0427(9) Uani 1 1 d . . .
O10 O 0.13807(13) 0.08150(12) 0.0712(2) 0.0600(12) Uani 1 1 d . . .
O11 O 0.29452(11) 0.07496(9) 0.1471(2) 0.0449(10) Uani 1 1 d . . .
O12 O 0.34038(14) 0.0000 0.3141(3) 0.0462(14) Uani 1 2 d S . .
O13 O 0.40825(15) 0.0000 0.1236(4) 0.0550(16) Uani 1 2 d S . .
O14 O 0.18079(11) 0.08144(10) 0.1767(3) 0.0565(12) Uani 1 1 d . . .
O15 O 0.34497(15) 0.11434(15) 0.3433(3) 0.0762(16) Uani 1 1 d D . .
H15 H 0.360(2) 0.128(2) 0.330(6) 0.114 Uiso 1 1 d D . .
O16 O 0.07298(16) 0.0000 0.1219(4) 0.0674(19) Uani 1 2 d S . .
O17 O 0.1188(3) 0.08347(19) 0.2048(6) 0.111(2) Uani 1 1 d . . .
O18 O 0.14120(18) 0.0000 0.3162(4) 0.075(2) Uani 1 2 d S . .
O19 O 0.29475(11) 0.08725(11) 0.2879(3) 0.0530(11) Uani 1 1 d . . .
O20 O 0.0893(2) 0.13679(15) 0.2924(4) 0.111(2) Uani 1 1 d . . .
O21 O 0.24121(18) 0.0000 0.3752(4) 0.0634(18) Uani 1 2 d S . .
B1 B 0.20871(19) 0.06545(19) 0.2107(4) 0.0479(17) Uani 1 1 d . . .
B2 B 0.27613(19) 0.06935(19) 0.2219(4) 0.0459(16) Uani 1 1 d . . .
B3 B 0.14511(19) 0.06968(18) 0.1530(4) 0.0479(17) Uani 1 1 d . A .
B4 B 0.1307(3) 0.0622(3) 0.0000 0.057(3) Uani 1 2 d S . .
B5 B 0.3294(2) 0.09594(17) 0.2807(4) 0.0442(16) Uani 1 1 d . . .
B6 B 0.3535(2) 0.0655(2) 0.0000 0.038(2) Uani 1 2 d S . .
B7 B 0.33273(18) 0.06821(16) 0.1460(4) 0.0386(14) Uani 1 1 d . . .
V6 V 0.0000 0.13336(3) 0.40861(8) 0.0406(4) Uani 1 2 d S . .
V7 V 0.0000 0.37197(3) 0.40665(8) 0.0378(3) Uani 1 2 d S . .
V8 V 0.0000 0.32512(3) 0.26835(8) 0.0465(4) Uani 1 2 d S . .
V9 V 0.0000 0.17859(3) 0.26984(9) 0.0617(5) Uani 1 2 d S . .
V10 V 0.0000 0.25346(4) 0.21922(9) 0.0615(5) Uani 1 2 d S . .
O31 O 0.03335(15) 0.36687(13) 0.5000 0.0418(13) Uani 1 2 d S . .
O32 O 0.03230(16) 0.21783(10) 0.2587(3) 0.0647(14) Uani 1 1 d . . .
O33 O 0.03354(11) 0.34627(9) 0.3422(2) 0.0425(9) Uani 1 1 d . . .
O34 O 0.07856(12) 0.30240(10) 0.3524(3) 0.0556(12) Uani 1 1 d . . .
O35 O 0.03224(15) 0.13945(12) 0.5000 0.0420(13) Uani 1 2 d S . .
O36 O 0.03391(14) 0.28699(10) 0.2578(3) 0.0568(12) Uani 1 1 d . . .
O37 O 0.03373(13) 0.15885(9) 0.3455(2) 0.0519(11) Uani 1 1 d . . .
O38 O 0.09256(13) 0.35599(10) 0.2858(3) 0.0563(12) Uani 1 1 d . . .
O39 O 0.11830(18) 0.35172(12) 0.1568(3) 0.0829(18) Uani 1 1 d D . .
H39 H 0.122(2) 0.3715(9) 0.140(4) 0.124 Uiso 1 1 d D . .
O40 O 0.08603(11) 0.35385(12) 0.5702(2) 0.0519(11) Uani 1 1 d . . .
O41 O 0.08545(14) 0.19431(11) 0.3187(3) 0.0711(14) Uani 1 1 d . . .
O42 O 0.08463(16) 0.25172(11) 0.2786(4) 0.0826(18) Uani 1 1 d . . .
O43 O 0.0000 0.41103(15) 0.3800(4) 0.0687(19) Uani 1 2 d S . .
O44 O 0.08576(12) 0.15642(12) 0.4302(3) 0.0726(15) Uani 1 1 d . . .
O45 O 0.09139(16) 0.30391(11) 0.2113(3) 0.0731(16) Uani 1 1 d . . .
O46 O 0.0000 0.34715(14) 0.1868(4) 0.087(3) Uani 1 2 d S . .
O47 O 0.0000 0.09365(13) 0.3831(4) 0.0574(16) Uani 1 2 d S . .
O48 O 0.0000 0.15715(17) 0.1869(4) 0.093(3) Uani 1 2 d S . .
O49 O 0.0000 0.25248(18) 0.1194(5) 0.120(4) Uani 1 2 d S . .
B11 B 0.0726(3) 0.28623(19) 0.2773(5) 0.062(2) Uani 1 1 d . A .
B12 B 0.0724(2) 0.33941(17) 0.3552(5) 0.0506(18) Uani 1 1 d . . .
B13 B 0.0998(3) 0.3368(2) 0.2185(4) 0.062(2) Uani 1 1 d D A .
B14 B 0.0670(3) 0.2212(2) 0.2835(5) 0.067(3) Uani 1 1 d . A .
B15 B 0.0683(2) 0.3574(2) 0.5000 0.038(2) Uani 1 2 d S . .
B16 B 0.0684(3) 0.1505(2) 0.5000 0.050(3) Uani 1 2 d S . .
B17 B 0.0719(3) 0.16213(19) 0.3470(5) 0.062(2) Uani 1 1 d . A .
C1A C 0.0859(5) 0.0991(3) 0.3228(10) 0.086(4) Uani 0.632(10) 1 d P A 1
H1A1 H 0.0872 0.0983 0.3827 0.103 Uiso 0.632(10) 1 calc PR A 1
H1A2 H 0.0626 0.0894 0.3058 0.103 Uiso 0.632(10) 1 calc PR A 1
C2A C 0.1163(4) 0.0787(3) 0.2863(7) 0.073(3) Uani 0.632(10) 1 d P A 1
H2A1 H 0.1390 0.0856 0.3122 0.087 Uiso 0.632(10) 1 calc PR A 1
H2A2 H 0.1125 0.0542 0.2976 0.087 Uiso 0.632(10) 1 calc PR A 1
C1B C 0.0700(8) 0.1056(6) 0.2721(17) 0.086(4) Uani 0.368(10) 1 d P A 2
H1B1 H 0.0494 0.1088 0.2351 0.103 Uiso 0.368(10) 1 calc PR A 2
H1B2 H 0.0639 0.0909 0.3189 0.103 Uiso 0.368(10) 1 calc PR A 2
C2B C 0.1216(10) 0.0932(7) 0.2112(18) 0.073(3) Uani 0.368(10) 1 d P A 2
H2B1 H 0.1264 0.1079 0.1638 0.087 Uiso 0.368(10) 1 calc PR A 2
H2B2 H 0.1422 0.0937 0.2489 0.087 Uiso 0.368(10) 1 calc PR A 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O12 V1 O1 107.32(19) . .
O12 V1 O1 107.32(19) . 11
O1 V1 O1 80.4(2) . 11
O12 V1 O2 109.33(19) . 11
O1 V1 O2 143.35(17) . 11
O1 V1 O2 88.62(16) 11 11
O12 V1 O2 109.33(19) . .
O1 V1 O2 88.62(16) . .
O1 V1 O2 143.35(17) 11 .
O2 V1 O2 79.6(2) 11 .
O12 V1 V3 106.6(2) . .
O1 V1 V3 126.08(12) . .
O1 V1 V3 126.08(12) 11 .
O2 V1 V3 40.62(11) 11 .
O2 V1 V3 40.62(11) . .
O12 V1 V2 108.4(2) . .
O1 V1 V2 40.43(11) . .
O1 V1 V2 40.43(11) 11 .
O2 V1 V2 123.60(12) 11 .
O2 V1 V2 123.60(12) . .
V3 V1 V2 145.00(6) . .
O13 V2 O1 109.4(2) . 11
O13 V2 O1 109.4(2) . .
O1 V2 O1 81.7(2) 11 .
O13 V2 O3 109.7(2) . 11
O1 V2 O3 88.20(15) 11 11
O1 V2 O3 140.74(19) . 11
O13 V2 O3 109.7(2) . .
O1 V2 O3 140.74(19) 11 .
O1 V2 O3 88.20(15) . .
O3 V2 O3 76.1(2) 11 .
O13 V2 V1 111.4(2) . .
O1 V2 V1 41.05(10) 11 .
O1 V2 V1 41.05(10) . .
O3 V2 V1 122.63(14) 11 .
O3 V2 V1 122.63(14) . .
O13 V2 V2 107.9(2) . 10
O1 V2 V2 122.98(11) 11 10
O1 V2 V2 122.98(11) . 10
O3 V2 V2 38.65(11) 11 10
O3 V2 V2 38.65(11) . 10
V1 V2 V2 140.64(3) . 10
O21 V3 O2 109.5(2) . .
O21 V3 O2 109.5(2) . 11
O2 V3 O2 81.8(2) . 11
O21 V3 O4 108.0(2) . 11
O2 V3 O4 142.33(18) . 11
O2 V3 O4 88.44(17) 11 11
O21 V3 O4 108.0(2) . .
O2 V3 O4 88.44(17) . .
O2 V3 O4 142.33(18) 11 .
O4 V3 O4 77.4(2) 11 .
O21 V3 V1 107.0(2) . .
O2 V3 V1 41.74(11) . .
O2 V3 V1 41.74(11) 11 .
O4 V3 V1 126.48(12) 11 .
O4 V3 V1 126.48(12) . .
O21 V3 V4 103.8(2) . .
O2 V3 V4 125.36(12) . .
O2 V3 V4 125.36(12) 11 .
O4 V3 V4 39.71(12) 11 .
O4 V3 V4 39.71(12) . .
V1 V3 V4 149.22(6) . .
O18 V4 O5 109.2(2) . 11
O18 V4 O5 109.2(2) . .
O5 V4 O5 82.7(2) 11 .
O18 V4 O4 109.1(2) . .
O5 V4 O4 141.68(17) 11 .
O5 V4 O4 87.10(17) . .
O18 V4 O4 109.1(2) . 11
O5 V4 O4 87.10(17) 11 11
O5 V4 O4 141.68(17) . 11
O4 V4 O4 78.5(2) . 11
O18 V4 V5 110.8(3) . .
O5 V4 V5 41.59(12) 11 .
O5 V4 V5 41.59(12) . .
O4 V4 V5 122.74(12) . .
O4 V4 V5 122.74(12) 11 .
O18 V4 V3 105.2(3) . .
O5 V4 V3 124.44(13) 11 .
O5 V4 V3 124.44(13) . .
O4 V4 V3 40.23(11) . .
O4 V4 V3 40.23(11) 11 .
V5 V4 V3 144.02(6) . .
O16 V5 O5 110.2(2) . .
O16 V5 O5 110.2(2) . 11
O5 V5 O5 82.4(2) . 11
O16 V5 O7 108.7(2) . 11
O5 V5 O7 141.00(19) . 11
O5 V5 O7 87.07(18) 11 11
O16 V5 O7 108.7(2) . .
O5 V5 O7 87.07(18) . .
O5 V5 O7 141.00(19) 11 .
O7 V5 O7 77.9(3) 11 .
O16 V5 V4 112.2(3) . .
O5 V5 V4 41.45(11) . .
O5 V5 V4 41.45(11) 11 .
O7 V5 V4 122.35(16) 11 .
O7 V5 V4 122.35(16) . .
O16 V5 V5 106.7(2) . 10
O5 V5 V5 122.76(12) . 10
O5 V5 V5 122.76(12) 11 10
O7 V5 V5 39.60(14) 11 10
O7 V5 V5 39.60(14) . 10
V4 V5 V5 141.12(4) . 10
B7 O1 V2 131.9(3) . .
B7 O1 V1 128.7(4) . .
V2 O1 V1 98.53(16) . .
B2 O2 V3 133.4(4) . .
B2 O2 V1 128.9(4) . .
V3 O2 V1 97.64(17) . .
B6 O3 V2 128.57(11) . 10
B6 O3 V2 128.57(11) . .
V2 O3 V2 102.7(2) 10 .
B1 O4 V4 131.2(4) . .
B1 O4 V3 127.6(4) . .
V4 O4 V3 100.06(19) . .
B3 O5 V4 130.7(4) . .
B3 O5 V5 132.4(4) . .
V4 O5 V5 96.96(18) . .
B1 O6 B2 134.0(6) . .
B4 O7 V5 129.01(16) . 10
B4 O7 V5 129.01(16) . .
V5 O7 V5 100.8(3) 10 .
B6 O8 B7 127.0(5) . .
B5 O9 B7 118.7(5) . .
B4 O10 B3 129.2(6) . .
B2 O11 B7 117.1(4) . .
B1 O14 B3 132.3(5) . .
B5 O15 H15 115(7) . .
C2B O17 C2A 84(5) . .
C2B O17 B3 109(6) . .
C2A O17 B3 126.4(10) . .
B5 O19 B2 120.8(5) . .
C1B O20 B17 118.6(12) . .
C1B O20 C1A 40.7(12) . .
B17 O20 C1A 113.5(7) . .
O6 B1 O14 120.0(6) . .
O6 B1 O4 121.0(6) . .
O14 B1 O4 119.0(6) . .
O6 B2 O11 110.0(5) . .
O6 B2 O19 110.5(5) . .
O11 B2 O19 109.7(5) . .
O6 B2 O2 110.8(5) . .
O11 B2 O2 108.9(5) . .
O19 B2 O2 106.9(5) . .
O17 B3 O10 108.3(7) . .
O17 B3 O5 107.1(6) . .
O10 B3 O5 110.3(5) . .
O17 B3 O14 110.6(7) . .
O10 B3 O14 108.2(6) . .
O5 B3 O14 112.2(5) . .
O7 B4 O10 124.4(5) . .
O7 B4 O10 124.4(5) . 10
O10 B4 O10 111.2(10) . 10
O19 B5 O9 123.3(5) . .
O19 B5 O15 118.0(6) . .
O9 B5 O15 118.7(6) . .
O8 B6 O8 118.7(8) . 10
O8 B6 O3 120.6(4) . .
O8 B6 O3 120.6(4) 10 .
O11 B7 O1 111.1(5) . .
O11 B7 O8 109.1(5) . .
O1 B7 O8 113.0(5) . .
O11 B7 O9 107.8(4) . .
O1 B7 O9 109.7(5) . .
O8 B7 O9 105.9(4) . .
O47 V6 O37 111.2(2) . 12
O47 V6 O37 111.2(2) . .
O37 V6 O37 82.3(3) 12 .
O47 V6 O35 108.7(2) . .
O37 V6 O35 139.89(19) 12 .
O37 V6 O35 87.11(19) . .
O47 V6 O35 108.7(2) . 3_556
O37 V6 O35 87.11(19) 12 3_556
O37 V6 O35 139.89(19) . 3_556
O35 V6 O35 76.6(3) . 3_556
O47 V6 V9 112.6(2) . .
O37 V6 V9 41.49(14) 12 .
O37 V6 V9 41.49(14) . .
O35 V6 V9 122.51(13) . .
O35 V6 V9 122.51(13) 3_556 .
O47 V6 V6 105.1(2) . 10_556
O37 V6 V6 122.91(13) 12 10_556
O37 V6 V6 122.91(13) . 10_556
O35 V6 V6 39.17(13) . 10_556
O35 V6 V6 39.17(13) 3_556 10_556
V9 V6 V6 142.22(4) . 10_556
O43 V7 O33 110.5(2) . 12
O43 V7 O33 110.5(2) . .
O33 V7 O33 81.1(2) 12 .
O43 V7 O31 108.1(3) . .
O33 V7 O31 141.32(19) 12 .
O33 V7 O31 88.09(17) . .
O43 V7 O31 108.1(3) . 3_556
O33 V7 O31 88.09(18) 12 3_556
O33 V7 O31 141.32(19) . 3_556
O31 V7 O31 77.5(3) . 3_556
O43 V7 V8 112.8(3) . .
O33 V7 V8 40.78(12) 12 .
O33 V7 V8 40.78(12) . .
O31 V7 V8 122.63(14) . .
O31 V7 V8 122.63(14) 3_556 .
O43 V7 V7 106.0(3) . 10_556
O33 V7 V7 123.44(12) 12 10_556
O33 V7 V7 123.44(12) . 10_556
O31 V7 V7 39.35(13) . 10_556
O31 V7 V7 39.35(13) 3_556 10_556
V8 V7 V7 141.15(3) . 10_556
O46 V8 O33 107.4(2) . .
O46 V8 O33 107.4(2) . 12
O33 V8 O33 80.7(2) . 12
O46 V8 O36 109.7(2) . 12
O33 V8 O36 142.97(17) . 12
O33 V8 O36 87.95(18) 12 12
O46 V8 O36 109.7(2) . .
O33 V8 O36 87.95(18) . .
O33 V8 O36 142.97(17) 12 .
O36 V8 O36 80.2(3) 12 .
O46 V8 V10 106.6(2) . .
O33 V8 V10 125.90(12) . .
O33 V8 V10 125.90(12) 12 .
O36 V8 V10 41.01(14) 12 .
O36 V8 V10 41.01(14) . .
O46 V8 V7 108.4(2) . .
O33 V8 V7 40.59(12) . .
O33 V8 V7 40.59(12) 12 .
O36 V8 V7 123.05(14) 12 .
O36 V8 V7 123.05(14) . .
V10 V8 V7 144.94(6) . .
O48 V9 O37 109.9(2) . 12
O48 V9 O37 109.9(2) . .
O37 V9 O37 81.3(3) 12 .
O48 V9 O32 109.3(2) . .
O37 V9 O32 140.72(18) 12 .
O37 V9 O32 88.5(2) . .
O48 V9 O32 109.3(2) . 12
O37 V9 O32 88.5(2) 12 12
O37 V9 O32 140.72(18) . 12
O32 V9 O32 75.8(3) . 12
O48 V9 V6 110.7(3) . .
O37 V9 V6 41.01(13) 12 .
O37 V9 V6 41.01(13) . .
O32 V9 V6 123.64(15) . .
O32 V9 V6 123.64(15) 12 .
O48 V9 V10 105.7(3) . .
O37 V9 V10 124.14(12) 12 .
O37 V9 V10 124.14(12) . .
O32 V9 V10 38.82(16) . .
O32 V9 V10 38.82(16) 12 .
V6 V9 V10 143.65(6) . .
O49 V10 O36 110.2(2) . 12
O49 V10 O36 110.2(2) . .
O36 V10 O36 81.9(3) 12 .
O49 V10 O32 108.4(2) . 12
O36 V10 O32 88.4(2) 12 12
O36 V10 O32 141.2(2) . 12
O49 V10 O32 108.4(2) . .
O36 V10 O32 141.2(2) 12 .
O36 V10 O32 88.4(2) . .
O32 V10 O32 76.1(3) 12 .
O49 V10 V8 107.4(3) . .
O36 V10 V8 41.89(14) 12 .
O36 V10 V8 41.89(14) . .
O32 V10 V8 126.42(15) 12 .
O32 V10 V8 126.42(15) . .
O49 V10 V9 104.5(3) . .
O36 V10 V9 124.32(14) 12 .
O36 V10 V9 124.32(14) . .
O32 V10 V9 38.97(15) 12 .
O32 V10 V9 38.97(15) . .
V8 V10 V9 148.04(7) . .
B15 O31 V7 129.02(13) . .
B15 O31 V7 129.02(13) . 10_556
V7 O31 V7 101.3(3) . 10_556
B14 O32 V10 128.0(5) . .
B14 O32 V9 129.1(5) . .
V10 O32 V9 102.2(3) . .
B12 O33 V7 130.4(4) . .
B12 O33 V8 130.0(4) . .
V7 O33 V8 98.64(19) . .
B11 O34 B12 116.5(5) . .
B16 O35 V6 128.86(13) . .
B16 O35 V6 128.86(13) . 10_556
V6 O35 V6 101.7(3) . 10_556
B11 O36 V10 134.2(4) . .
B11 O36 V8 128.7(4) . .
V10 O36 V8 97.1(2) . .
B17 O37 V6 133.8(5) . .
B17 O37 V9 128.6(4) . .
V6 O37 V9 97.5(2) . .
B13 O38 B12 118.3(5) . .
B13 O39 H39 138(4) . .
B15 O40 B12 126.8(5) . 10_556
B14 O41 B17 128.8(7) . .
B14 O42 B11 132.7(7) . .
B16 O44 B17 130.5(6) . .
B13 O45 B11 120.3(5) . .
O34 B11 O42 111.2(7) . .
O34 B11 O45 111.3(6) . .
O42 B11 O45 108.0(6) . .
O34 B11 O36 109.6(6) . .
O42 B11 O36 109.3(6) . .
O45 B11 O36 107.3(7) . .
O40 B12 O34 110.9(6) 10_556 .
O40 B12 O33 113.2(5) 10_556 .
O34 B12 O33 109.1(5) . .
O40 B12 O38 107.3(5) 10_556 .
O34 B12 O38 108.8(5) . .
O33 B12 O38 107.4(5) . .
O45 B13 O39 118.0(6) . .
O45 B13 O38 123.9(6) . .
O39 B13 O38 118.1(6) . .
O32 B14 O42 121.6(8) . .
O32 B14 O41 121.6(7) . .
O42 B14 O41 116.7(9) . .
O40 B15 O40 119.3(8) . 10_556
O40 B15 O31 120.3(4) . .
O40 B15 O31 120.3(4) 10_556 .
O44 B16 O44 118.2(9) 10_556 .
O44 B16 O35 120.9(5) 10_556 .
O44 B16 O35 120.9(5) . .
O37 B17 O41 115.1(7) . .
O37 B17 O44 110.5(5) . .
O41 B17 O44 108.0(7) . .
O37 B17 O20 111.5(7) . .
O41 B17 O20 103.6(6) . .
O44 B17 O20 107.7(7) . .
C2A C1A O20 107.9(10) . .
C2A C1A H1A1 110.1 . .
O20 C1A H1A1 110.1 . .
C2A C1A H1A2 110.1 . .
O20 C1A H1A2 110.1 . .
H1A1 C1A H1A2 108.4 . .
O17 C2A C1A 111.8(11) . .
O17 C2A H2A1 109.3 . .
C1A C2A H2A1 109.3 . .
O17 C2A H2A2 109.3 . .
C1A C2A H2A2 109.3 . .
H2A1 C2A H2A2 107.9 . .
O20 C1B C2B 81.8(15) . .
O20 C1B H1B1 115.0 . .
C2B C1B H1B1 115.0 . .
O20 C1B H1B2 115.0 . .
C2B C1B H1B2 115.0 . .
H1B1 C1B H1B2 112.0 . .
O17 C2B C1B 96(6) . .
O17 C2B H2B1 112.6 . .
C1B C2B H2B1 112.6 . .
O17 C2B H2B2 112.6 . .
C1B C2B H2B2 112.6 . .
H2B1 C2B H2B2 110.1 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
V1 O12 1.621(5) .
V1 O1 1.951(4) .
V1 O1 1.951(4) 11
V1 O2 1.959(4) 11
V1 O2 1.959(4) .
V1 V3 2.9165(18) .
V1 V2 2.9385(18) .
V2 O13 1.619(5) .
V2 O1 1.927(4) 11
V2 O1 1.927(4) .
V2 O3 1.976(3) 11
V2 O3 1.976(3) .
V2 V2 3.086(3) 10
V3 O21 1.595(7) .
V3 O2 1.916(4) .
V3 O2 1.916(4) 11
V3 O4 2.004(4) 11
V3 O4 2.004(4) .
V3 V4 3.0558(19) .
V4 O18 1.643(6) .
V4 O5 1.934(4) 11
V4 O5 1.934(4) .
V4 O4 1.983(4) .
V4 O4 1.983(4) 11
V4 V5 2.9003(19) .
V5 O16 1.630(6) .
V5 O5 1.939(4) .
V5 O5 1.939(4) 11
V5 O7 2.006(4) 11
V5 O7 2.006(4) .
V5 V5 3.091(3) 10
O1 B7 1.456(7) .
O2 B2 1.506(8) .
O3 B6 1.391(10) .
O3 V2 1.976(3) 10
O4 B1 1.407(9) .
O5 B3 1.466(8) .
O6 B1 1.323(8) .
O6 B2 1.430(8) .
O7 B4 1.245(14) .
O7 V5 2.006(4) 10
O8 B6 1.339(6) .
O8 B7 1.493(8) .
O9 B5 1.364(8) .
O9 B7 1.516(7) .
O10 B4 1.426(9) .
O10 B3 1.452(8) .
O11 B2 1.431(8) .
O11 B7 1.454(8) .
O14 B1 1.342(8) .
O14 B3 1.466(9) .
O15 B5 1.389(8) .
O15 H15 0.81(2) .
O17 C2B 0.41(3) .
O17 C2A 1.363(14) .
O17 B3 1.413(11) .
O19 B5 1.347(8) .
O19 B2 1.472(8) .
O20 C1B 1.46(3) .
O20 B17 1.493(9) .
O20 C1A 1.570(14) .
B4 O10 1.426(9) 10
B6 O8 1.339(6) 10
V6 O47 1.615(5) .
V6 O37 1.919(4) 12
V6 O37 1.919(4) .
V6 O35 1.947(4) .
V6 O35 1.947(4) 3_556
V6 V9 2.899(2) .
V6 V6 3.018(3) 10_556
V7 O43 1.595(6) .
V7 O33 1.930(4) 12
V7 O33 1.930(4) .
V7 O31 1.993(4) .
V7 O31 1.993(4) 3_556
V7 V8 2.9326(19) .
V7 V7 3.083(3) 10_556
V8 O46 1.600(6) .
V8 O33 1.937(4) .
V8 O33 1.937(4) 12
V8 O36 1.971(4) 12
V8 O36 1.971(4) .
V8 V10 2.929(2) .
V9 O48 1.608(6) .
V9 O37 1.937(5) 12
V9 O37 1.937(5) .
V9 O32 1.967(5) .
V9 O32 1.967(5) 12
V9 V10 3.057(2) .
V10 O49 1.648(8) .
V10 O36 1.936(5) 12
V10 O36 1.936(5) .
V10 O32 1.960(5) 12
V10 O32 1.960(5) .
O31 B15 1.359(11) .
O31 V7 1.993(4) 10_556
O32 B14 1.368(12) .
O33 B12 1.493(9) .
O34 B11 1.412(9) .
O34 B12 1.472(8) .
O35 B16 1.421(12) .
O35 V6 1.947(4) 10_556
O36 B11 1.482(11) .
O37 B17 1.433(10) .
O38 B13 1.370(8) .
O38 B12 1.519(8) .
O39 B13 1.364(9) .
O39 H39 0.839(19) .
O40 B15 1.343(6) .
O40 B12 1.450(9) 10_556
O41 B14 1.389(11) .
O41 B17 1.440(8) .
O42 B14 1.371(9) .
O42 B11 1.428(9) .
O44 B16 1.343(7) .
O44 B17 1.487(11) .
O45 B13 1.334(9) .
O45 B11 1.471(9) .
B12 O40 1.450(9) 10_556
B15 O40 1.343(6) 10_556
B16 O44 1.343(7) 10_556
C1A C2A 1.517(17) .
C1A H1A1 0.9900 .
C1A H1A2 0.9900 .
C2A H2A1 0.9900 .
C2A H2A2 0.9900 .
C1B C2B 2.23(4) .
C1B H1B1 0.9900 .
C1B H1B2 0.9900 .
C2B H2B1 0.9900 .
C2B H2B2 0.9900 .
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 -0.006 -0.002 -0.042 15134 2957 ' '
